Characterization of the pressure-induced second-order phase transition in the mixed-valence vanadate BaV~6~O~11~
Friese, Karen; Kanke, Yasushi; Grzechnik, Andrzej; Acta Crystallographica Section B 65 (2009) 326–333; doi:10.1107/S010876810901444X

data_2104359
_publ_section_title
;
 Characterization of the pressure-induced second-order phase transition
 in the mixed-valence vanadate BaV~6~O~11~
;
_journal_coeditor_code           EB5003
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              326
_journal_page_last               333
_journal_paper_doi               10.1107/S010876810901444X
_journal_volume                  65
_journal_year                    2009
_chemical_formula_sum            'Ba O11 V6'
_chemical_formula_weight         619
_chemical_name_common            Bariumvanadate
_chemical_name_systematic        ' ?'
_space_group_IT_number           186
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   5.775(3)
_cell_length_b                   5.775(3)
_cell_length_c                   13.238(4)
_cell_measurement_reflns_used    684
_cell_measurement_temperature    293
_cell_measurement_theta_max      28.5
_cell_measurement_theta_min      3.07
_cell_volume                     382.3(3)
_computing_cell_refinement       X-Area
_computing_data_collection       X-Area
_computing_data_reduction        'Jana2006, Absorb V6.1'
_computing_publication_material
'Jana2006 (Petricek, Dusek & Palatinus, 2006)'
_computing_structure_refinement
'Jana2006 (Petricek, Dusek & Palatinus, 2006)'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.74
_diffrn_measurement_device_type  IPDS-2T
_diffrn_measurement_method       \omega-scans
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0622
_diffrn_reflns_av_sigmaI/netI    0.1421
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            1016
_diffrn_reflns_reduction_process Jana2006
_diffrn_reflns_theta_full        25.61
_diffrn_reflns_theta_max         27.96
_diffrn_reflns_theta_min         3.08
_exptl_absorpt_coefficient_mu    12.14
_exptl_absorpt_correction_T_max  0.2182
_exptl_absorpt_correction_T_min  0.1726
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   Jana2006
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.375(4)
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             564
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.06
_refine_diff_density_max         2.69
_refine_diff_density_min         -1.92
_refine_ls_extinction_coef       0
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_ref   0.75
_refine_ls_number_constraints    5
_refine_ls_number_parameters     17
_refine_ls_number_reflns         229
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0891
_refine_ls_R_factor_gt           0.0284
_refine_ls_shift/su_max          0.0070
_refine_ls_shift/su_mean         0.0023
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0193
_refine_ls_wR_factor_ref         0.0253
_reflns_number_gt                108
_reflns_number_total             229
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            eb5003.cif
_cod_data_source_block           III
_cod_original_sg_symbol_Hall     'P 6c;-2c'
_cod_original_formula_sum        'Ba1 O11 V6'
_cod_database_code               2104359